- Email: [email protected]

A multiscale micromechanics-hydration model for the early-age elastic properties of cement-based materials Olivier Bernard, Franz-Josef Ulm*, Eric Lemarchand Massachusetts Institute of Technology, Cambridge, MA 02139, USA Received 1 May 2002; accepted 13 January 2003

Abstract The E-modulus of early age cement-based materials, and more importantly, its evolution in time, is one of the most critical material-tostructural design parameters affecting the likelihood of early-age concrete cracking. This paper addresses the problem by means of a multistep micromechanics approach that starts at the nanolevel of the C – S – H matrix, where two types of C – S – H develop in the course of hydration. For the purpose of homogenization, the volume fractions of the different phases are required, which are determined by means of an advanced kinetics model of the four main hydration reactions of ordinary portland cement (OPC). The proposed model predicts with high accuracy the aging elasticity of cement-based materials, with a minimum intrinsic material properties (same for all cement-based materials), and 11 mixdesign specific model parameters that can be easily obtained from the cement and concrete suppliers. By way of application, it is shown that the model provides a quantitative means to determine (1) the solid percolation threshold from micromechanics theory, (2) the effect of inclusions on the elastic stiffening curve, and (3) the development of the Poisson’s ratio at early ages. The model also suggests the existence of a critical water-to-cement ratio below which the solid phase percolates at the onset of hydration. The development of Poisson’s ratio at early ages is found to be characterized by a water-dominated material response as long as the water phase is continuous, and then by a soliddominated material response beyond the solid percolation threshold. These model-based results are consistent with experimental values for cement paste, mortar, and concrete found in the open literature. D 2003 Elsevier Ltd. All rights reserved. Keywords: Concrete; Hydration; Elastic moduli; Micromechanics; Percolation threshold

1. Introduction The elastic or Young’s modulus (E-modulus) of concrete is important in all structures that are subjected to boundary conditions of displacements that are more or less restrained. Its importance is further amplified when the deformation is restrained from a very young age on pavements, dams, concrete slabs of composite structures, massive parts poured in successive layers, etc., for which the E-modulus, and more importantly its evolution in time, is one of the most critical material-to-structural mechanical design parameters affecting the likelihood of early-age concrete cracking (see reviews by, e.g., Refs. [1– 3]). The E-modulus, in effect, evolves substantially with the hardening of the material and * Corresponding author. Tel.: +1-617-253-3544; fax: +1-617-2536044. E-mail address: [email protected] (F.-J. Ulm). URL: http://cist.mit.edu. 0008-8846/03/$ – see front matter D 2003 Elsevier Ltd. All rights reserved. doi:10.1016/S0008-8846(03)00039-5

increases continuously from zero to a value near its service value. It has long been recognized that this early-age concrete stiffening, which is often referred to as ‘aging elasticity,’ cannot be described as a simple function of time. In fact, the kinetics of this stiffening is related to the hydration reactions of the material, which are thermally activated. This brought about macroscopic approaches, in which the evolution of the E-modulus was described by the maturity concept [4– 8] or the hydration degree [9– 12] or the solidification degree [13]. It has been shown that the maturity degree and the hydration degree are thermodynamically equivalent macroscopic state variables [14]. The hydration degree concept has been widely used in many large-scale engineering applications, ranging from innovative bridge design [15,16], shotcrete tunnel engineering [17 – 19], to concrete dam engineering [20,21]. Still, the macroscopic hydration degree concept is only a first step towards a comprehensive materials-to-

1294

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

structural engineering design approach, which aims at optimizing the structural performance of early-age concrete structures by means of an appropriate material choice. Recent progress in experimental mechanics, particularly in nanoindentation techniques, makes it possible to assess the elastic properties at very fine scales [22,23] and to upscale this elastic behavior to larger scales by means of advanced homogenization methods: cement paste [23], mortar, and concrete [24 –27]. To our knowledge, this approach has been only employed for hardened cement-based materials, and there is still a missing link between the physical chemistry of cement hydration and the micro- to macromechanics of cement-based materials. The goal of this paper is to close this gap by modeling the aging elasticity of early-age concrete composites. The originality of the proposed approach relies on use of a multistep micromechanical homogenization procedure that starts at the nanolevel of the C –S – H matrix, along with a physical chemistry model for the kinetics of the four main hydration reactions of ordinary portland cement (OPC) that determine the volume fractions of the involved mechanically active phases.

2. Elements of continuum micromechanics Concrete is a fairly complex heterogeneous composite material, with a random microstructure at different length scales ranging from the nanometer scale to the macroscopic decimeter scale. Continuum micromechanics offers a framework to address this heterogeneity. The underlying idea of continuum micromechanics is that it is possible to separate a heterogeneous material into phases with on-average constant material properties. The three elements of continuum micromechanics are (see, e.g., Ref. [28]): 1. Representation, which deals with the geometrical description of the considered heterogeneous material system. Representation includes the identification of the different phases in a representative element volume V (r.e.v.), and their morphology. A phase, in the sense of continuum micromechanics, is not necessarily a material phase as used in physical chemistry, but a material domain that can be identified at a given scale with a homogeneous deformation state that is with constant material properties. 2. Localization, which establishes the link between a microscopic on-average constant strain (or stress state), prescribed at the boundary @V of the r.e.v., and the strain state (or stress state) in the individual (homogeneous) phases composing the r.e.v. 3. Homogenization, which is based on volume averaging over the r.e.v. of the constitutive relations defined at the scale of the phases. Homogenization delivers the macroscopic properties of the r.e.v. as a function of the

microscopic phase properties, their volume fractions, and their specific morphologies. Application of these three elements to cement-based materials at early ages is detailed below. 2.1. Representation of the multiscale microstructure of early-age concrete The heterogeneity of cement-based material manifests itself at different scales. For purpose of mechanical analysis, the microstructure can be broken down into four elementary levels, as sketched in Fig. 1 [23]: 1. The lowest level (Level I) we consider is the one of the C – S– H matrix that forms at early ages by the hydration of C3S and C2S.1 This level of a characteristic length scale of 108 – 106 m is the smallest material length scale that is, at present, accessible by mechanical testing, i.e., nanoindentation. For this reason, lower scales, which are investigated by, e.g., quasi-elastic neutron scattering [29], will not be considered here. At the considered Level I, it now well established that the C – S– H exist in at least two different forms with different volume fractions [30] and elastic properties [22,23]. The morphology of the two types of C – S –H is correlated with two different processes of hydration of clinker compounds. During the early stages of hydration, nucleation and growth of C – S – H occurs at the surface of the cement grains, leading to the softer outer products. With hydration progressing (t>20 h for C3S, see Ref. [31], for temperature effect, see, e.g., Ref. [29]), the cement grains are covered by a growing layer of C –S – H, and the hydration is controlled by the diffusion process through this layer. While outer products are still formed, new C – S –H is primarily formed in a space confined by the existing C –S – H layer; and these new C –S – H have a higher density, leading to an on-average higher stiffness of the inner product C –S – H. Many labels have been devised in cement chemistry for the two types of C –S – H in cement-based materials: OP – C – S – H and IP – C – S – H for Outer and Inner Products [32 – 34], Middle Product and Late Product [35,36], Groundmass and Phenograins [37], or more recently LD – C – S– H and HD –C – S –H for low-density and high-density C – S –H [30,38]. From a mechanical point of view, however, only average stiffness values of these two types of C –S – H are accessible by nanoindentation, that is, mean stiffness values for low-density and high-density C – S – H [23], which include the nanoporosity (or C – S –H gel porosity) and eventually some fine calcium hydroxide crystals intimately mixed with the gels. We refer to these two types of C– S –H as 1 The cement’s chemistry abbreviations will be used in this paper (C3S=3CaOSiO2, C2S=2CaOSiO2, C3A=3CaOAl2O3, C4AF=4CaO Al2O3Fe2O3).

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

1295

Fig. 1. Multiscale microstructure of cement-based materials, adapted from Ref. [23].

phases in a micromechanical sense, as detailed before; that is, each C – S – H phase is associated with a homogeneous deformation state and homogeneous mechanical properties. This mechanical definition of the C – S – H phases, which is consistent with the nanoindentation results, justifies the use of a neutral labeling of these two types of C – S– H phases as C –S – Ha phase and C – S– Hb phase, associated, respectively, with the outer and inner products, or low-density and high-density products. From a morphological point of view, the C – S –H matrix can be considered as a twophase material, composed of a stiffer inclusion phase (C –S – Hb phase) embedded into a softer matrix phase (C –S – Ha phase). At early ages, the volume fractions of these two phases depend on the progress of the C3S and C2S – clinker hydration. This level is the starting point for the homogenization approach developed in this paper. 2. The C – S –H matrix, together with unhydrated cement products (i.e., the four clinker phases C3S, C2S, C3A, C4AF), large portlandite crystals (CH=Ca(OH)2), aluminates (see exact formulations in Ref. [35]), and macroporosity in the case of high water-to-cement ratio materials (roughly w/c>0.4 [39]) forms the cement paste and is referred to as Level II (106 – 104 m). At early ages, it is the scale of the solid percolation threshold. More precisely, when OPC is mixed with water, the solid phases (clinker) of the composite material are discontinuous. The freshly mixed material can be considered as a pure viscous liquid with nonappreciable shear modulus [40]. The solid phase is then built up through random growth of hydration products, mainly due to the formation of C – S– H at the surface of cement grains.

Once the solid phases become connected, the composite material at level II can support appreciable shear stresses. Following percolation theory, this set point is generally referred to as the solid percolation threshold [41,42]. At the micrometer scale, this percolation threshold is considered to be a material property that is mainly affected by the w/c ratio and the cement fineness. It is one focus of this paper to derive this percolation threshold from micromechanics theory. More precisely, from a morphological point of view, a transformation occurs during hydration from a highly disordered microstructure without any phase dominating, to a matrix-inclusion morphology. Once the C – S –H phase percolates, the composite cement paste consists of inclusions (clinker phases, A-phase, CH phase and porosity) embedded into a C –S – H matrix. 3. Level III (103 – 102 m) refers to mortar; that is a threephase composite material composed of a cement paste matrix, sand particle inclusions, and an interfacial transition zone (ITZ). This scale has been focus of micromechanical modeling attempts, both analytically (e.g., Refs. [27,43]) and numerically (e.g., Refs. [26,42]). For early-age concrete, there is a critical lack of data concerning the development of mechanical properties of the ITZ; related, e.g., to a higher CH concentration. In this paper, in a first approach, we will not consider the ITZ, but will reduce the three-phase composite material to a two-phase material composed of spherical inclusions of sand particles (<2 mm) embedded in a continuous matrix of homogenized cement paste. In this case, the important volume fractions are those of the inclusion and of the matrix, and they are fixed in time.

1296

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

4. Concrete as a composite material is considered on Level IV (102 –101 m). Similar to Level III, homogenization approaches that consider at this scale a three-phase material composed of aggregates (>2 mm) embedded in a continuous homogeneous mortar matrix and an ITZ have been developed [42,43]. For early-age concrete, we restrict the analysis to a two-phase system composed of aggregates and mortar, and the required volume fractions are also fixed in time. It is worth noting that the four levels described above respect the separability of scale condition; that is, each scale is separated by the next one by at least one order of length magnitude. This is a prerequisite for the application of continuum micromechanics [28].

ization is a constant strain in all phases, that is, er=E () Ar=I, which forms the basis of so-called mixture theories. This localization condition, however, fails to describe the different strain distribution in the microstructure, which depends on stiffness and morphology of the different phases. In a refined approach, the strain localization tensor is estimated from the linear elastic solution of some idealized geometrical configurations. The most common one that applies best to the morphology encountered at all different levels of cement-based materials, is the Eshelbian-type ellipsoidal inclusion embedded in a reference medium [44], for which an estimate Arest of the localization tensor is given in the form [28]: Esh Aest : ðC1 : Cr IÞ 1 r ¼ ½I þ Sr 0

: h½I þ SEsh : ðC1 : Cr IÞ 1 i1 V r 0

2.2. Localization The breakdown of the multiscale heterogeneous microstructure of cement-based materials into the four-level microstructure, separated on average by one or several order of length magnitude, allows us to consider each level as r.e.v., V, composed of n homogeneous phases (in a micromechanical sense) of constant material properties per phase, P and volume fraction fr=Vr/V, such that r=1,n fr=1. Following continuum micromechanics, each level is considered to be subjected to a macroscopic strain prescribed at the boundary @V of the r.e.v. This homogeneous boundary condition, which is often referred to as Hashin-type boundary condition, reads: on @V : uðxÞ ¼ E x

ð1Þ

where u is the microscopic displacement vector, x denotes the position vector at the microscopic scale, and E is the macroscopic strain tensor in V; the symbol ‘‘’’ stands for scalar product. The macroscopic strain tensor E is related to the microscopic strain e(x) by the volume-averaging relation: Z 1 E ¼ heðxÞiV ¼ eðxÞdV ð2Þ V V It is assumed in linear continuum micromechanics that the macroscopic strain E can be linked to the microscopic strain er by means of a linear strain localization condition: er ¼ Ar : E

ð3Þ

where Ar is a fourth-order localization or concentration tensor (as it concentrates a macroscopic quantity prescribed at the boundary into a microscopic phase), which obeys to the consistency condition (combination of Eqs. (2) and (3)): E ¼ her iV ¼ hAr : EiV () hAr iV ¼ I

ð5Þ

where C0 is the tensor of elastic moduli of the reference medium, Cr is the fourth-order elasticity tensor of phase r=1,n, and SrEsh is the Eshelby tensor of phase r, which depends on C0, the geometry, and the orientation of phase r. Given the random microstructure of cement-based materials, it is naturally to consider all phases as isotropic and the inclusions as spherical. The first assumption implies the isotropy of the local and the reference medium, that is: Cr ¼ 3kr J þ 2mr K;

C0 ¼ 3k0 J þ 2m0 K

ð6Þ

where kr, mr, k0, and m0 are the bulk moduli and the shear moduli of phase r and of the reference medium, respectively; Jijkl=(1/3)dijdkl is the volumentric part of the fourth-order unit tensor I, and K=IJ is the deviator part; dij stands for the Kronecker delta. The second assumption of spherical inclusions implies the following form of the Eshelby tensor SEsh for phase r: r est SEsh ¼ aest r 0 J þ b0 K

ð7Þ

with aest 0 ¼

3k0 ; 3k0 þ 4m0

best 0 ¼

6ðk0 þ 2m0 Þ 5ð3k0 þ 4m0 Þ

ð8Þ

2.3. Homogenization and choice of reference medium To homogenize the local material properties, constitutive relations are required for the different phases, together with the volume-averaging relation linking the microscopic stress sr and the macroscopic stress ; analogously to Eq. (2): ¼ hsðxÞiV

ð9Þ

ð4Þ

The symbol ‘‘:’’ stands for double contraction. I is the fourth-order unit tensor. The simplest form of strain local-

Use in Eq. (9) of a linear elastic constitutive law for each microscopic phase, i.e., of the form sr=Cr : er, together with the strain localization condition (Eq. (3)),

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

i.e., sr=(Cr : Ar) : E, delivers the following linear homogenization formula for the macroscopic (or homogenized) elasticity tensor Chom: ¼ Chom : E; Chom ¼ hCr : Ar iV ¼

X

fr Cr : Ar

ð10Þ

r

While expression (10) is an exact theoretical definition of Chom, the practical determination of Chom is generally based on estimates of the localization tensor for each phase Aest r . It is readily understood that the quality of the homogenization result is intimately related to the quality of the localization condition. For instance, use of Aest r =I (which comes to assume the same strain in all phases and macroscopically) delivers the Voigt upper bound (or mixture rule), 8r; Aest r

¼

I; Cest hom

¼ hCr : IiV ¼

X

fr Cr

ð11Þ

1297

are taken into account in the localization and homogenization procedure. For the four-level upscaling procedure, we consider: (1) The Mori –Tanaka scheme [45], in which the matrix phase is chosen as reference medium, i.e., C0Cm. The MT scheme is appropriate for materials that exhibit a strong matrix-inclusion morphology and mechanical interactions in between particles. This scheme is chosen for the two-phase spherical inclusion composites at Level I, Level III, and Level IV, for which Eqs. (14) and (15) reduce to: est khom kI =km 1 ¼ 1 þ fI 1 þ aest km ð1 fI ÞðkI =km 1Þ m

ð16Þ

mest mI mm hom ¼ 1 þ fI est mm 1 þ bm ð1 fI ÞðmI =mm 1Þ

ð17Þ

r

In a refined analysis, considering the Eshelbian-type strain localization (Eq. (5)), the following estimate of the est macroscopic (or homogenized) elasticity tensor Chom is obtained:

and Eq. (8) to:

est aest 0 am ¼

3km ; 3km þ 4mm

est best 0 bm ¼

6ðkm þ 2mm Þ 5ð3km þ 4mm Þ ð18Þ

Esh : ðC1 : Cr IÞ 1 iV Cest hom ¼ hCr : ½I þ Sr 0

: h½I þ SEsh : ðC1 : Cr IÞ 1 i1 V r 0

ð12Þ

Substituting Eqs. (6) –(8) into Eq. (12) yields explicit expressions for the homogenized bulk modulus and shear modulus: est est Cest hom ¼ 3khom J þ 2mhom K

est khom

¼

X r

f r kr 1 þ

aest 0

ð13Þ kr 1 k0

1

"

1 #1 X est kr fr 1 þ a0 1 k0 r

mest hom ¼

X r

ð14Þ est Ehom ¼

1 mr fr mr 1 þ best 1 0 m0

1 #1 X est mr f r 1 þ b0 1 m0 r

(2) The self-consistent scheme [46,47], in which the reference medium coincides with the homogenized medium, est C0Chom . The SCS describes well materials characterized by perfect disorder (polycrystal). Being related to percolation theory, it allows one to account for a percolation threshold. The SCS, therefore, is chosen for Level II homogenization to account for a solid percolation threshold. In contrast to the MT scheme, the SCS involves the solution of two nonlinear equations (Eqs. (14) and (15)), in which est est k0khom ; m0mhom . Finally, for the purpose of comparison with experimental data, the homogenized Young’s modulus and Poisson’s ratio at each level are evaluated from:

"

est est est 9khom mhom 3khom 2mest est hom ; n ¼ hom est est 3khom þ mest 6khom þ 2mest hom hom

ð19Þ

3. Input parameters ð15Þ

To close the upscaling procedure, we need to choose the appropriate reference medium, in which the inclusions are embedded. This choice is important as it determines the level of interaction between inclusions and special physical features such as the percolation threshold that

The four-level upscaling scheme requires, at each level, input of the shear and bulk moduli, kr=1,n and mr=1,n, and of the volume fractions of the involved phases, fr=1,n. The est est output, khom and mhom , at each level serves as the input for the next level. Table 1 summarizes the input – output structure of the four-level upscaling scheme. The mechanical, chemical, and mix-design input parameters are detailed below.

1298

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

Table 1 Input – output structure of the four-level upscaling scheme Level

I: C – S – H matrix C – S – Ha C – S – Hb II: Cement paste C – S – H matrix C3S – Clinker C2S – Clinker C3A – Clinker C4AF – Clinker CH Aluminates Water Voids III: Mortar CP – matrix Sand (<2 mm) IV: Concrete Mortar-matrix Aggregate (>2 mm)

Input

Output

Mechanical

Chemical

ka, ma kb, mb

fa fb=1fa

kCest– S – H , mCest– S – H kC3S, mC3S kC2S, mC2S kC3A, mC3A kC4AF, mC4AF kCH, mCH kA, mA – –

fC – S – H

MixDesign MT scheme kCest– S – H , mCest– S – H SCS scheme est est kCP , mCP

fC3S fC2S fC3A fC4AF fCH fA fw fv

ques by Velez et al. [51]. Unfortunately, there is a lack of data on the elastic properties of aluminates. It is reasonable to assume that these properties are similar to the elastic properties of the C –S – H matrix, obtained by the first-level upscaling procedure. Levels III and IV: The elastic stiffness of sand and aggregates are well known (see for instance Ref. [52]) and are typically provided by the aggregate supplier. These mechanical input parameters are considered to be time independent. 3.2. Chemical input parameters

est est , mCP kCP ks, ms

fCP=1fs fs

est est kM , mM kg, mg

fM=1fg fg

MT scheme est est kM , mM MT scheme kCest, mest C

3.1. Mechanical input parameters: nanoindentation data Recent progress in instrumented nanoindentation provides a fairly consistent amount of data for the mechanical input parameters of the model (see Table 2):

The second set of input parameters is the set of volume fractions occupied by the different phases in the r.e.v. at Level I and Level II. Given that the phases form via the four elementary hydration reactions, it is natural to determine the volume fractions from cement chemistry. This requires two steps: (1) determination of the hydration degree of each reaction from reaction kinetic laws and (2) consideration of the volume change associated with each reaction. 3.2.1. Hydration kinetics model It is common practice in physical chemistry (see, e.g., Atkins [53]) to describe the kinetics of hydration of each clinker phase X (X=C3S, C2S, C3A, and C4AF) by nucleation and growth kinetic laws that link the reaction rate dxX/dt to the driving force for the chemical reaction, called the affinity

Level I: Acker [22] and Constantinides and Ulm [23] provided values for the mean elastic stiffness of the two C –S – H phases at Level I. The values, which were obtained for two different types of cement pastes and with different sharp indenters, coincide, suggesting that the values are intrinsic material parameters that do not depend on mix proportioning. That what differs, at this scale, from one cement paste to another is the volume fraction of the two phases, which depends on the mix proportioning. Given the scale which is accessible by nanoindentation, the stiffness value for each C – S– H phase includes both the solid phase and the nanoscale gel porosity within the C – S –H. Level II: Beaudoin [48] and Wittmann [49] measured the elastic modulus of CH compacts on specimens with different porosities. The elastic modulus of these compacts was obtained from three-point bending tests. The intrinsic modulus of CH was found by extrapolating to zero porosity, logE versus porosity curves. The order of magnitude of these values was confirmed by nanoindentation results by Acker [22] and Constantinides and Ulm [23], which also lie within the bounds determined by Monteiro and Chang [50]. The stiffness of the clinker phases (C3S, C2S, C3A, C4AF) were determined by indentation by Acker [22] and by extrapolation techni-

Table 2 Intrinsic elastic properties of cement paste constituents Level I: C – S – H matrix C – S – Ha

C – S – Hb

II: Cement paste C3S – Clinker C2S – Clinker C3A – Clinker C4AF – Clinker CH

E (GPa)

n (–)

20±2 21.7±2.2

0.24

31±4 29.4±2.4

0.24

135±7 147±5 140±10 130±20 160±10 145±10 125±25 35.24 48 39.77 – 44.22

0.3 0.3 0.3 0.3

0.305 – 0.325

36±3 38±5 Values in bold are used in the homogenization procedure.

References Acker [22] Constantinides and Ulm [23] Acker [22] Constantinides and Ulm [23]

Acker [22] Velez et al. [51] Acker [22] Velez et al. [51] Acker [22] Velez et al. [51] Velez et al. [51] Beaudoin [48] Wittmann [49] Monteiro and Chang [50] Acker [22] Constantinides and Ulm [23]

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

1299

Table 3 Reaction kinetic model parameters of the four clinker hydration reactions (from Refs. [31,35]) Clinker

C3S

C2S

C3A

C4AF

w/c

Avrami model

0.3 0.5 0.7 0.3 0.5 0.7 0.3 0.5 0.7 0.3 0.5 0.7

Diffusion model

tX(T0) [h]

k [1]

xX,0 [1]

D [cm /h]

* [1] xX

Activation energy EaX/R [K]

13.5 11.9 10.5 71.2 60.9 58.6 57.7 49.2 35.9 27.0 21.4 14.3

1.86 1.72 1.66 1.10 0.96 0.84 1.14 1.00 0.86 2.44 2.30 2.16

0.02

0.60

4500

0.00

0.421010 2.641010 15.61010 6.641013

0.60

2500

0.04

2.641010

0.60

5500

0.40

0.421010 2.641010 15.61010

0.60

4200

2

Values for other w/c ratio are linearly interpolated.

A (xX), in addition to any kinetics constant that determines the time scale of the chemical reaction. These kinetic laws can be written in the following dimensionless form: tX

dxX ˜ XÞ ¼ Aðx dt

ð20Þ

where tX is the characteristic time associated with the reaction, and A˜ (xX) is a normalized affinity. Given the thermal activation of the hydration reaction, the characteristic time depends on the temperature, and this dependency is well described, for cement hydration, by the Arrhenius concept: tX ðT Þ ¼ tX ðT0 Þexp

EaX R

1 1 T0 T

ð21Þ

where EaX is the activation energy of the chemical reaction, R the universal gas constant, and tX(T0) is the characteristic time of the reaction at a constant reference temperature T0 (typically, T0=293 K). The expression of the normalized affinity depends on the physical process at stake. For the cement hydration, there are (at least) three processes [35]. (1) Dissolution of the clinker phases during the induction period. Given the relatively short period, the process can be simulated by a constant reaction rate; that is, A˜ =1 and tX=tX,0=tX,0/xX,0, where tX,0 is the duration of the induction period, and xX,0 is the degree of hydration threshold of clinker X at the end of the induction period. (2) Nucleation and growth-controlled hydration of the clinker phases, which is the focus of, e.g., the Avrami model [54], commonly employed in cement chemistry. Expressed in the form of the kinetic law (Eq. (20)), the normalized affinity of the Avrami model reads (see derivation in Appendix): A˜A ðxX Þ ¼

ð1 dxX Þ 1

ðlnð1 dxX ÞÞ k 1

dxX ¼ hxX xX;0 iþ > 0

for ð22Þ

and the characteristic time: tX ðT0 Þ ¼

1 kk

ð23Þ

where hxi+ denotes the positive part of x. The exponent k defines the reaction order, and k is the rate constant. The Avrami parameters, k, and xX,0, together with the kinetic parameters tX(T0) and EaX/R, are well established by now (see, e.g., Berliner et al. [31]), even though some coefficients may vary from one author to the other (see also Ref. [55]). The values used in this paper are taken from Ref. [31] and are summarized in Table 3. (3) Beyond a critical hydration degree x*X , which corresponds to a critical thickness of hydration products formed around the clinker grains, the kinetics of the hydration reactions is limited by diffusion of dissolved ions through the layers of hydrates formed around the clinker. The problem has been addressed by several authors by means of diffusion theory [31,56]. We refer to the works of Fuji and Kondo [56]. Written in the rate form of kinetic law (Eq. (20)), the normalized affinity of this process can be expressed as: 2

A˜ D ðxX Þ ¼

ð1 xX Þ 3 1

1

ð1 xX*Þ 3 ð1 xX Þ 3

for xX > xX*

ð24Þ

and the characteristic time by: tX ðT0 Þ ¼

R2 3D

ð25Þ

where D is a diffusion coefficient (of dimension [D]=L2/T), and R is the average initial radius of clinker grains. The model parameters, x*X and D, of the diffusion-type kinetics law of the different clinker phases are extracted from the works of Berliner et al. [31] and Taylor [35]. They are summarized in Table 3. The values of the kinetic parameters in Table 3 have been determined for an OPC of a fineness f0=3602 cm2/g and an average particle size R=5104 cm. Given that the hydra-

1300

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

Table 4 Input parameters for the determination of the volume fractions (level I and level II) Reactants 3 r(*) X [g/cm ]

MX [g/mol] qCX– S – H [1] X qCH [1] X [1] qw X qV [1]

Products

C3S mC S rc P 3 mX

C2S mC S rc P 2 mX

C3A mC A rc P 3 mX

C4AF mC AF rc P 4 mX

X

X

X

X

228.32 1.0 1.3 5.3 0.073

172.24 1.0 0.3 4.3 0.077

270.20 – – 10.0

430.12 – – 10.75

tion kinetics is accelerated by a smaller fineness due to the greater specific surface area, the values of the characteristic time determined from Eq. (25) are corrected by: tX ðT0 ; fÞ ¼

f0 tX ðT0 ; f0 Þ f

ð26Þ

The hydration kinetics model is then complete. Finally, it is useful to recall the relation between the clinker hydration degrees xX and the overall hydration degree x(t) of cement-based material systems [57,35]: P mX xX ðtÞ xðtÞ ¼ X P ð27Þ mX X

where mX=mC3S, mC2S, mC3A, and mC4AF are the mass fractions of the clinker phases in the cement, which are generally provided by the cement producer, based on a chemical analysis of the cement (see, e.g., Taylor [35]). For instance, the mass fraction of C3S in OPC is typically mC3S=0.6. 3.2.2. Volume fractions Level I The hydration kinetics model determines the hydration degree of each clinker phase, which is required for the determination of the volume fractions of the phases involved in the micromechanics model. At Level I, the two types of C – S – H are the reaction products of the hydration of C3S and C2S. If we accept that the low-density C – S– Ha phase corresponds to the outer products, and the high-density C – S –Hb phase to the inner products, it is natural to assume that the first are formed during the nucleation and growth process (xXx*X), and the second during the diffusion-controlled hydration reaction, that is:

w

c

1.00

C–S–H

3.15

18 – – – –

– – – – –

2.04

227.2 – – – –

CH 2.24

74 – – – –

where VCC–3SS – H and VCC–2SS – H are asymptotic values of the volume occupied by the reaction products of the hydration of C3S and C2S in the C – S –H r.e.v. VC – S – H =VCC–3SS – H + VCC–2SS – H VCC–3SS – H (resp. VCC–2SS – H ) can be determined in a dimensionless form from: C3 S rC*3 S =M C3 S VCSH C3 S ¼ qCSH ; 0 Vc rCSH =M CSH

rC*3 S ¼

M C3 S mC S ¼ rc P 3 Vc0 mX

ð30Þ

X

C2 S rC*2 S =M C2 S VCSH C2 S ¼ qCSH ; 0 Vc rCSH =M CSH

rC*2 S ¼

M C2 S mC S ¼ rc P 2 0 Vc mX

ð31Þ

X

qCC3–SS – H =nC – S – H/nC3 S

where =1 and qCC2–SS – H =nC – S – H/nC2S= 1 express that nC3 S =1 mol of C3S (resp. nC2 S =1 mol of C2S) is required for the formation of nC – S – H=1 mol of C –S – H; V c0 is the initial cement volume, r*C3S (resp. r*C2S) is the apparent mass density of C3S (resp. C2S) in cement (mass density rc); MC3S, MC2S=molar mass of C3S and C2S, such that r*C3S /MC3S=number of moles of C3S per unit volume of cement, and analogously, rC – S – H/MC – S – H=number of moles of C –S – H per unit volume of C –S – H (rC – S – H=mass density of C – S –H; MC – S – H=molar mass of C – S– H). The input values for the determination of VCC–3SS – H and VCC–2SS – H are given in Table 4. Finally, the relative volume fractions at level I of the two types of C – S– H are then obtained from: fa ¼

Va ; Va þ Vb

fb ¼

Vb ¼ 1 fa Va þ Vb

ð32Þ

C S

3 Va ðtÞ ¼ VCSH ðxC*3 S hxC*3 S xC3 S ðtÞiþ Þ

C S

2 þ VCSH ðxC*2 S hxC*2 S xC2 S ðtÞiþ Þ

ð28Þ

C S

3 Vb ðtÞ ¼ VCSH hxC3 S ðtÞ xC*3 S iþ

C S

2 þ VCSH hxC2 S ðtÞ xC*2 S iþ

ð29Þ

Fig. 2 displays, as a function of the hydration degree, x, the evolution of the volume fractions of the two types of C –S – H for a w/c=0.5 cement paste. At complete hydration (x=1), the model predicts fa0.7 and fb0.3, which is in perfect agreement with the volume fractions determined analytically by Tennis and Jennings [30] based on specific surface measurements and experimentally by Constantinides and

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

1301

qCw3 S =(4+1.3)/1=5.3; analogously, qCw2 S =(4+0.3)/1=4.3; qwC3A=10 and qwC4AF=10.75; see Table 4. On the product side, the volume occupied by the C – S –H matrix, VC – S – H=Va+Vb, is defined by Eqs. (28) and (29), C3 S C2 S xC3 S ðtÞ þ VCSH xC2 S ðtÞ VCSH ðtÞ ¼ VCSH

ð36Þ

where VCC–3SS – H and VCC–2SS – H are defined by Eqs. (30) and (31). Analogously, the volume occupied by the Portlandite, CH, is a combination of the reaction products of the hydration of C3S and C2S: C3 S C2 S xC3 S ðtÞ þ VCH xC2 S ðtÞ VCH ðtÞ ¼ VCH C 3S

ð37Þ

C 2S

where VCH and VCH are the asymptotic volume contributions of the C3S and C2S hydration to the CH formation:

Fig. 2. Influence of the cement fineness on the evolution of the volume fractions of the two types of C – S – H phases for a w/c=0.5 OPC paste (Level I).

Ulm [23] based on a statistical analysis of nanoindentation results. The evolution of the two types of C –S – H for a finer cement (f=6000 cm2/g) are also presented in Fig. 2. In such conditions, the volume fraction of C –S – Hb is divided by 2 at the end of the hydration. 3.2.3. Volume fractions Level II Level II is composed of both reactants and products. On the reactant side, the volume occupied by the four clinker phases is linearly related to the clinker hydration degree, that is: VX ðtÞ ¼

VX0 ð1

xX ðtÞÞ;

VX0 mX ¼P 0 Vc mX

ð33Þ

C3 S r* =M C3 S VCH C3 S ¼ qCH C3 S ; 0 Vc rCH =M CH C3 S r* =M C2 S VCH C2 S ¼ qCH C2 S 0 Vc rCH =M CH

ð38Þ

C 3S

where qCH =nCH/nC3S=1.3 (i.e, hydration of nC3S=1 mol of C3S leads to the formation of nCH=1.3 mol of CH); CS qCH2 =nCH/nC2S=0.3, and rCH/MCH=number of moles per unit volume of CH (rCH=mass density of CH; MCH=molar mass of CH; see Table 4). Finally, during the hydration of the clinker phases, capillary voids are created due to a negative volume balance (or chemical shrinkage) between reactant and product phases involved in the hydration reactions of the clinker phases: VV ðtÞ ¼

X

DVVX xX ðtÞ;

X

DVVX mX ¼ qX VP Vc0 mX

X

where VX0 is the initial volume of the clinker phases in the cement. The other reactant phase is water, which is consumed in the four hydration reactions: X Vw ðtÞ ¼ Vw0 VwX xX ðtÞ 0 ð34Þ X

Vw0

is the initial volume of water in the mix, and VwX is the volume of water that is consumed in the clinker hydration reaction (complete hydration), which is given by: VwX r*X =M X ¼ qX ; w Vc0 rw =M w

r*X ¼

MX mX ¼ rc P Vc0 mX

ð35Þ

X

where qwX =nw/nX denotes the number nw of moles of water consumed during the hydration of nX=1 mol of clinker phase X of apparent mass density r*X. For instance, in the hydration of nC3S=1 mol of C3S, 4 mol of water are fixed by the formation of C – S– H (1.1 mol are chemically bound, 2.9 mol are absorbed in the C – S –H pores), and 1.3 mol of water are involved in the hydration of C3S to form CH; thus,

ð39Þ

X

According to Taylor [35], qCV3S=0.073; qCV2S= qVC3A = see Table 4. The total volume of the r.e.v. at Level II is the sum of the volumes of both reactant and product phases, that is: X VII ¼ Vw ðtÞ þ VX ðtÞ qCV4AF=0.077;

X |ﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄ{zﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄ ﬄ} Reactants

þ VCSH ðtÞ þ VCH ðtÞ þ VA ðtÞ þ VV ðtÞ |ﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄ{zﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄﬄ}

ð40Þ

Products

where VA(t) is the volume occupied by the aluminates. The volume of the r.e.v. is constant in time and can therefore be evaluated from the initial volume of the cement and water in the mixture: r w VII ¼ Vc0 þ Vw0 ¼ Vc0 1 þ c ð41Þ rw c where V c0 is the initial volume of cement, rc/rw is the cement-to-water mass density ratio, and w/c is the water-to-

1302

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

cement ratio. Eqs. (33) – (41) form a set of equations that allows determination of the volume fractions for the Level II homogenization (see Table 1): fCSH fw ¼

Va þ Vb ¼ ; VII

Vw ; VII

fv ¼

VX fX ¼ ; VII

Vv VII

fCH

VCH ¼ ; VII ð42Þ

P and fA ¼ 1 ðfCSH þ X fx þ fCH þ fw þ fv Þ. Note that the initial volume of cement disappears from the determination of the (dimensionless) volume fractions, reducing the number of input parameters to the w/c ratio, the mass fraction of the clinker phases in the cement, and a set of chemical constants summarized in Table 4. By way of example, Fig. 3 displays, as a function of the overall hydration degree x, the evolution of the volume fractions at Level II for a Type I OPC paste: w/c=0.5, mC3S=0.543, mC2S=0.187, mC3A=0.076, mC4AF=0.073. At complete hydration, the four clinkers are all consumed ( fX=0); fC – S – H=53.8%, fCH=15.6%, and fA=16.9%. The remaining water, fw=6.2%, and the formed voids, fv=7.5%, form the macro-porosity fw+fv=13.7%, which is consistent with the results of Hansen [39]. The total porosity is the sum of the intrinsic C – S – H gel porosity and aluminates of approximately 28% and the capillary porosity fw+fv=13.7%, i.e., 41.7%, which is close to the value of 39.7±1.1% measured by drying at 105C, on the same material by Constantinides and Ulm [23].

Table 5 Set of material-specific model parameters required to calculate the input parameters of the proposed model Cement

Concrete

f [cm2/g] mC3S [1] mC2S [1] mC3A [1] mC4AF [1]

c [kg/m3] w/c [1] s [kg/m3] g [kg/m3]

Es=g [GPa] ns=g [1]

the water content w=rwfw0 (kg/m3), the sand contents s=rs fs0 (kg/m3) (<2 mm, Level III), and the aggregate content g=rg fg0 (kg/m3) (>2 mm, Level IV), where rc=3.15 g/cm3, rw=1.00 g/cm3, rs=rg=2.65 g/cm3 are the mass densities of cement, water, sand, and aggregate which occupy the volume fractions f c0, f w0, f 0s , and f g0 in a reference volume. At this scale, the volume fractions of the two-phase hardening material are constant in time and are functions of only the mix-design parameters, i.e., at Level III: fs ¼

fs0 s=rs ¼ ; 0 0 0 fc þ fw þ fs c=rc þ w=rw þ s=rs

fCP ¼ 1 fs ð43Þ

where fs and fCP are the sand and cement paste volume fractions. Analogously, at Level IV: fg ¼

fc0

þ

fw0

fs0 g=rs ¼ ; þ fs0 þ fg0 c=rc þ w=rw þ ðs þ gÞ=rs

3.3. Mix-design input parameters

fM ¼ 1 fg

ð44Þ

The volume fractions at Levels III and IV are all related to mass proportions of the mix design. The mix proportions are commonly described by the mass of each constituent present in 1 m3 of mix: the cement content c=rc fc0 (kg/m3),

where fg and fM are the coarse aggregate and mortar volume fractions. In summary, the application of the proposed micromechanical model to a specific cement-based material requires 11 mix-design specific model parameters, summarized in Table 5, that can be easily obtained from the cement and concrete suppliers. The other model parameters, i.e., the mechanical parameters (Table 2) and the chemical kinetic parameters (Table 3) and chemical volume change parameters (Table 4), are intrinsic values, which are the same for all cement-based materials.

4. Validation and discussion

Fig. 3. Evolution of volume fractions of the phases of a w/c=0.5 cement paste (Level II).

The predictive capabilities of the model are shown in Fig. 4 in the form of a plot of predicted versus experimental Emodulus values for early-age cement paste, mortar, and concrete found in the open literature [8,12,23,27,40,52]. The individual data sets of the E-modulus evolution versus the hydration degree are shown in Figs. 5 –7, comparing results obtained from the micromechanical model with the experimental results. The input parameters for the validation sets are given in Tables 6 and 7. The model accurately

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

1303

Fig. 4. Predictive capability of the model: predicted versus measured Emodulus (data sets [8,12,23,27,40,52]).

Fig. 6. Comparison of predicted versus measured E-modulus of mortar (M1 [23], M2 [40]).

captures the early-age stiffness development of cementbased materials. There are three model features that deserve particular attention: (i) the percolation threshold, (ii) the role of aggregate inclusions on the macroscopic stiffness evolution, and (iii) the development of the Poisson’s ratio at early ages. These aspects are discussed below.

the percolation threshold of the SCS is associated with a volume fraction of the solid phases (i.e., the phases which exhibit a significant elasticity) greater than 50%, which is equivalent to a porosity smaller than 50%. From Eq. (42), the threshold can be written as: X x x0 () fCSH þ fX þ fCH þ fA 0:5; X

4.1. Percolation threshold

fw þ fv 0:5

One important model feature is the account of percolation threshold x0 through the use of the SCS scheme at Level II. This percolation threshold corresponds to the percolation of the solid phase, that is, the C –S – H matrix phase, the clinker phases, and the A-phase. More precisely,

Unfortunately, there are few experimental values of the percolation threshold reported in the open literature:

Fig. 5. Comparison of predicted versus measured E-modulus of cement paste (CP1 [23], CP2+CP3 [40]).

ð45Þ

De Schutter and Taerwe [12] determined the percolation threshold by extrapolating stiffness values measured at

Fig. 7. Comparison of predicted versus measured E-modulus of concrete (CO7+CO8 [8], CO9 [12], CO10 [27]).

1304

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

Table 6 Input parameters of validation set at levels I and II References

Type

f [cm2/g]

mC3S [1]

mC2S [1]

mC3A [1]

mC4AF [1]

w/c [1]

Constantinides and Ulm [23] Boumiz et al. [40]

CP1+M1 CP2 CP3 M2 M3

3602 7600 7600 7600 7600

0.543 0.663 0.663 0.638 0.620

0.187 0.121 0.121 0.089 0.113

0.076 0.106 0.106 0.082 0.083

0.073 0.009 0.009 0.062 0.060

0.50 0.35 0.40 0.52 0.39

CP4+CO1 CP5+CO2 CP6+CO3 CP7+CO4 CP8+CO5 CP9+CO6

3600 3600 3600 3600 3600 3600

0.645 0.560 0.560 0.560 0.686 0.686

0.130 0.180 0.180 0.180 0.050 0.050

0.060 0.052 0.052 0.052 0.068 0.068

0.115 0.110 0.110 0.110 0.087 0.087

0.54 0.58 0.48 0.48 0.56 0.61

CO7 CO8 CO9

3466 3466 5320

0.607 0.607 0.594

0.187 0.187 0.118

0.028 0.028 0.078

0.122 0.122 0.100

0.50 0.33 0.50

CO10

3466

0.607

0.187

0.028

0.122

0.42

Granger [52] Chooz Penly Flamanville Paluel CivauxB11 CivauxBHP Laplante [8] BO BTHP De Schutter and Taerwe [12] Le Roy [27] BO5

higher hydration degrees to zero-stiffness values. For a concrete prepared at w/c=0.5, they reported percolation threshold that varied between x0=0.17 and x0=0.25. These values are on the same order as the percolation threshold predicted by the micromechanical model (see CO9 in Fig. 7). Boumiz et al. [40] determined percolation thresholds by combining ultrasonic measurements with hydration heat measurements on cement pastes (CP2 w/c=0.35 and CP3 w/c=0.40, see Fig. 5) and mortars (M2 w/c=0.52, see Fig. 6). The time of percolation was set equal to the material age at which the first significant shear ultrasonic velocity was measured. Parallel hydration heat measurements allowed replacing the time by the hydration degree threshold x0. The values determined by this method differ from the ones predicted by the micromechanical model, mod exp for both cement paste (x0,CP2 =0.046 versus x0,CP2 =0.015;

mod mod =0.11 versus xexp x0,CP3 0 =0.021) and mortar (x0,M2 =0.246 exp versus x0,M2=0.015). The difference may well result from the relatively low solid volume fraction threshold (Eq. (45)) of the SC upscaling scheme, which could lead to an overestimation of the hydration degree percolation threshold x0. On the other hand, the difference may well be related to the experimental difficulty to accurately determine the hydration degree by calorimetric measurements in the very first hours of hydration, given that heat of hydration is only produced beyond the initial degree of hydration xX,0 of each clinker phase (see Table 3). In other words, the experimental error may well be on the order of Dx=0.03 –0.06, that is on the order of the difference between experimental and predicted percolation threshold.

Finally, it is interesting to note that the percolation threshold defined by Eq. (45) translates into a critical w/c

Table 7 Input parameters of validation set at levels III and IV References

Type

c [kg/m3]

s [kg/m3]

Es=g [GPa]

ns=g [1]

Constantinides and Ulm [23] Boumiz et al. [40]

CP1+M1 M2 M3

620 569 730

1241 1390 1297

– – –

50 45 45

0.30 0.30 0.30

CP4+CO1 CP5+CO2 CP6+CO3 CP7+CO4 CP8+CO5 CP9+CO6

350 350 375 375 350 266

836 752 795 772 772 879

1130 1012 1040 1048 1100 1133

70 65 55 65 61 61

0.27 0.27 0.22 0.27 0.28 0.28

CO7 CO8 CO9

342 398 300

670 709 670

1200 1216 1280

65 65 45

0.23 0.23 0.23

CO10

355

696

1204

75

0.23

Granger [52] Chooz Penly Flamanville Paluel CivauxB11 CivauxBHP Laplante [8] BO BTHP De Schutter and Taerwe [12] Le Roy [27] BO5

g [kg/m3]

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

ratio, below which the model predicts a zero percolation threshold, i.e., x0=0, for which fv(x=0)=0, and thus, fw (x=0)=f w0 0.5. Indeed, from Eqs. (34) and (41):

describes the mechanical activity of the clinker elasticity, that is: kXeff ¼ h kX ;

rc w 0 V w r c r w 0:5 ) w x0 ¼ 0 () fw0 ¼ w ¼ r w c c VII rc 1þ rw c ¼ 0:318 ð46Þ

For w=c > w=c ¼ 0:318, the percolation threshold x0 increases quasilinearly with the w/c ratio, as displayed in Fig. 8 (determined with the input parameter of CP1). While the value of the critical w/c ratio of w=c ¼ 0:318 is related to the relatively low solid volume fraction percolation threshold of the SCS, the dependence of x0 on w/c is consistent with percolation theory applied to cement-based materials [42] and experimental observations [12]. On the other hand, for w/c ratios smaller than w=c, the model considers that the unhydrated cement grains are initially in contact so that the solid phase percolates. This situation, however, never occurs in cement-based materials, in which superplasticizer prevents the grain-to-grain (dry) contact by coating the clinker surfaces. From a mechanical point of view, this coating deactivates the force transmission from clinker to clinker grain, thus neutralizing the mechanical contribution of the clinker elasticity to the overall elasticity. This coating effect, which is not related to the hydration reactions but to another chemophysical phenomenon, is not considered in our micromechanical model, and its consideration would require consideration of the coating activity of superplasticizer. This can be achieved, in a first approach, by means of an activation degree h2[0,1] that

Fig. 8. Influence of w/c ratio on the percolation threshold x0 (determined with input parameters of CP1; Experimental values from Refs. [12,40]).

1305

meff X ¼ h mX

ð47Þ

Initially h=0, and h!1 with the loss of the superplasticizer. The effect of this activation factor for a low w/c =0.33 concrete is shown in Fig. 7 (CO8). The hydration degree was determined with the proposed model, and h=H(ttr) was assumed in the micromechanical model, where H(x) is the Heaviside function, and tr=10 h, the retardation time of the setting process due to the use of superplasticizer. This adds a further input parameter to the model, but one that is independent of the hydration reactions. Finally, the percolation threshold x0 appears to have a strong influence on the asymptotic E-modulus reached when the hydration is completed or stopped due to a lack of water. With all other parameters constant, the model predicts that the smaller the percolation threshold, the higher the final E-modulus. For example, the final Emodulus of concrete CO8 (x0=0, w/c=0.33) in Fig. 7 is higher than the E-modulus of concrete CO10 (x0=0.12, w/ c=0.42), despite the lower stiffness of the inclusions of concrete CO8 (see Table 7), and the smaller final value of the hydration degree of CO8 (x1, CO8=0.77 versus, x1, CO10=0.97). Hence, it may be suggested from the micromechanical model that the well-known higher stiffness of low w/c ratio cement-based materials results from their lower percolation threshold x0. 4.2. Role of inclusions The model reveals an interesting feature of aging elasticity related to the presence of sand and aggregate in the composite at Levels III and IV, respectively. The E-modulus of cement paste, which represents the matrix at Level III, develops almost linearly with the hydration degree (see Fig. 5). By contrast, the addition of sand inclusions in mortar, and aggregates in concrete, leads to a deviation from this linear behavior of the paste: the modulus increases much stronger at early hydration degrees (‘‘elastic stiffening’’) but then levels off (see Figs. 6 and 7). The higher the inclusion volume fraction, the stronger this elastic stiffening following the percolation threshold x0. This stronger early-age stiffening also affects the final value. For instance, despite a 10% lower E-modulus of sand in mortar M2 over M1, the greater inclusion volume fraction of fs,M2=0.53 compared to fs,M1=0.48 leads to a 10% greater final E-modulus of M2 over M1 (see Fig. 6). Analogously, for concrete (see Fig. 7), the greater inclusion volume fraction of concrete CO9 of fs,CO9+fg,CO9=0.75 compared to fs,CO7+fg,CO7=0.71 of CO7 compensates the lower inclusion stiffness of Es=45 GPa of concrete CO9 compared to Es=65 GPa of CO7. These two effects, inclusion stiffness versus inclusion volume fraction, are in

1306

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

Fig. 9. Influence of inclusion stiffness Es and inclusion volume fraction fi=fs+fg on the E-modulus of concrete (calculated for x=1.0).

competition during the hydration process: for x0.4, the inclusion fraction fi=fs+fg seems to have a stronger influence than the E-modulus Es on the evolution of the composite E-modulus of cement-based materials, and for higher hydration degrees, it is the inverse. Fig. 9 displays the composite E-modulus as a function of the inclusion stiffness for different inclusion fractions. For a given set of mix parameters (here mix proportions of concrete CO9), a simple rule can be established: a decrease of 10% of the volume fraction of inclusions is roughly compensated by an increase of 10 GPa of the inclusion stiffness Es. Finally, we note that the micromechanical model employed at Levels III and IV slightly overestimates the stiffness value of the composite material, mortar, and concrete. This overestimation is due to the effect of the ITZ, which was not taken into account in the two-phase model. A three-phase model that considers the ITZ would be required to improve the accuracy of the proposed micromechanical model.

est =0.48 to roughly decrease of the Poisson’s ratio from nhom est nhom=0.15. After the percolation threshold, Byfors [5] and De Schutter and Taerwe [12] reported an increase of the Poisson’s ratio to a final value close to n=0.25; this increase has been attributed to the progressive hardening of the material. These experimental observations highlight the complex role played by the different components of cementbased materials on the shear-to-bulk modulus ratio, which est increases below the percolation threshold from mhom / est est est khom=0.04 to mhom /khom=0.91 and decreases beyond x0 to est est mhom /khom =0.60. To evaluate the role of water in the development of the Poisson’s ratio, two simulations were performed with the micromechanical model; one in which the compressibility of the water phase was considered (i.e., kw=2.18 GPa; mw=0), the other in which the compressibility was neglected (i.e., kw=mw=0.). The predicted development of the homoest genized Poisson’s ratio nhom for the two limit cases is displayed in Fig. 10. The simulations were carried out for the mix proportions of cement paste CP1 and mortar M1. We note:

When the compressibility of water is taken into account, est the effective Poisson’s ratio nhom is a continuously decreasing function of the hydration degree, and the rate of decrease is amplified by the presence of inclusions (mortar M1). Below the percolation threshold (x0=0.25), the model predicts for the cement paste a decrease from est est nhom =0.50 to nhom =0.37. This confirms qualitatively that the experimentally observed decrease of the Poisson’s ratio is due to the consumption of water in the early stages of the hydration reaction. This decrease is higher at lower w/c ratios. est When the compressibility of the water is neglected, nhom is a continuously increasing function of the hydration

4.3. Poisson’s ratio est The evolution of the Poisson’s ration nhom during the hydration of cement-based materials is related to the evolution of the effective shear modulus to bulk modulus ratio est est mhom /khom :

nest hom ¼

est 3 2mest hom =khom est est 6 þ 2mhom =khom

ð48Þ

est Given the negligible shear-to-bulk modulus ratio mhom / est khom!0 of water-dominated suspensions, it is generally accepted that the Poisson’s ratio of the fresh mix should be close to the Poisson’s ratio of water n=0.5 [12]. During the early stages of hydration, the experimental values of Boumiz et al. [40] and Byfors [5] provide evidence of a

Fig. 10. Evolution of Poisson’s ratio of cement paste CP1 and mortar M1 and influence of a reduced w/c ratio (CP1 with w/c=0.35).

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

degree. Beyond the percolation threshold, the model est est predicts an increase from nhom =0.20 to nhom =0.25, which is little affected by the presence of inclusions. This confirms that any increase of the Poisson’s ratio is associated with the solid stiffness evolution. As x approaches 1, both models converge towards an asymptotic value that is not affected by the compressibility of the remaining water in the mix, nor by the sand est inclusions. The value of nhom calculated for cement paste CP1 is in good agreement with the experimental value exp nhom =0.24 reported by Le Bellego [58] for similar cement-based materials. The two limiting cases studied here highlight the effect of the percolated phase on the effective shear-to-bulk modulus ratio and on the Poisson’s ratio. Below the percolation threshold, the water phase is continuous, and its bulk modulus, therefore, strongly affects the composite Poisson’s ratio. Beyond the percolation threshold, the solid phase is continuous and dominates the increase of the Poisson’s ratio of the composite. The ‘real’ evolution of the Poisson’s ratio lies within these limiting cases. Since our micromechanics model is based on only one solid percolation threshold, i.e., Eq. (45), it cannot capture the continuous transition from the water-dominated effective composite material behavior of the fluid suspension to the soliddominated effective composite material behavior of the hardening solid phase. Such a model requires consideration of a water percolation threshold in addition to the solid percolation threshold. It is suggested that once the water phase becomes discontinuous, the water bulk modulus kw ceases to affect the overall elasticity of the composite, marking the switch from a decreasing Poisson’s ratio to an increasing Poisson’s ratio.

5. Conclusions Continuum micromechanics combined with advanced cement chemistry hydration models provides a rational tool to study the aging elasticity of cement-based materials, with a minimum of intrinsic material properties (same for all cement-based materials), and 11 mix-design specific model parameters that can be easily obtained from the cement and concrete supplier. The key to the model is the four microstructure levels of cement-based composite materials, which allow the gap between the physical chemistry of cement hydration and the mechanics of cement-based materials to be bridged. We suggest: 1. The solid percolation threshold derived from micromechanics theory is a function of the w/c ratio. For the employed SCS, a critical w/c ratio of w=c ¼ 0:318 defines a zero percolation threshold. Below this value, the solid phase percolates at the onset of hydration, once the activity of superplasticizer ceases to coat the clinker

1307

phases. Beyond this value, the percolation threshold increases quasilinearly with increasing w/c ratio. This percolation threshold affects significantly the final stiffness value of the hardened cement-based material. 2. The two effects of sand and aggregate inclusions on the composite stiffness evolution relate to the inclusion volume fractions and inclusion stiffness. At early stages of hydration (around the percolation threshold), the first effect dominates over the latter, and for higher hydration degrees, it is the inverse. For a given set of mix parameters, a decrease of 10% of the volume fraction of inclusions can be compensated by an increase of 10 GPa of the inclusions E-modulus. This simple rule can be employed for a fine-tuned mix design of fast-stiffening or slow-stiffening early-age concrete that have the same final service state E-modulus. 3. The development of the Poisson’s ratio at early ages relates to (at least) two percolation thresholds: one for the water phase and one for the solid phase. As long as the water phase is continuous, the Poisson’s ratio decreases due to the consumption of water in the hydration reactions. When the water phase becomes discontinuous, the development of the Poisson’s ratio becomes dominated by the solid stiffening, leading to an increase of the Poisson’s ratio. Finally, a refinement of the model components on both the micromechanics side and the cement chemistry side can still improve the accuracy of the prediction of the model. For instance, on the micromechanics side, consideration of the ITZ at Levels III and IV will surely improve the predictive capabilities of the model, particularly for high w/c ratio mortars and concretes. On the cement chemistry side, an improved understanding of the effects of superplasticizers on the early stages of hydration will extend the domain of application of the model to very low w/c ratio cement-based materials.

Acknowledgements The authors gratefully acknowledge the financial support of this study by the Swiss National Science Foundation (SNF), mediated through the research committee of the Swiss Federal Institute of Technology in Lausanne, Switzerland, enabling the postdoctoral work of the first author at MIT. The authors also acknowledge the valuable review comments of the original manuscript. The detailed description of the Elements of continuum micromechanics in the revised version was suggested by one of the reviewers.

Appendix A. Kinetic laws This appendix shows the deviation of the normalized affinity expression (22) for the nucleation and growth

1308

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

kinetics based on Avrami’s model. The Avrami equation reads [54]: ln½1 ða a0 Þ ¼ ½kðt t0 Þ k

[9]

ð49Þ

where a is the degree of reaction at time t, k is the rate constant, and k is an exponent. The constants a0 and t0 define the degree of reaction and time at which the nucleation and growth kinetic regime begins. Differentiating Eq. (49) with respect to time, a rate expression as a function of time is obtained (see Ref. [55]): da ¼ mk k ðt t0 Þk1 exp½k k ðt t0 Þk dt

ð50Þ

[10]

[11]

[12]

[13]

Replacing the time tt0 by aa0 according to Eq. (49), the rate expression as a function of the reaction degree reads:

[14]

1 da ¼ kkð1 ða a0 ÞÞðlnð1 ða a0 ÞÞÞ1 k dt

[15]

ð51Þ

Expressed in the dimensionless form (Eq. (20)), we obtain: t

[16]

da ¼ A˜A ðaÞ dt

ð52Þ

where the normalized affinity A˜ A(a) and the characteristic time t read: A˜A ðaÞ ¼

1 ða a0 Þ ðlnð1 ða a0 ÞÞÞ

1 k 1

;

t¼

1 kk

[17]

[18]

ð53Þ

These are Eqs. (22) and (23), for which the constants are given in Table 3 determined from given values for k and k found in the literature [31]. Finally, expression (24) of the normalized affinity for the diffusion-controlled hydration kinetics is derived in an analogous way, using the integrated form of the solution of Fuji and Kondo [56].

[19]

[20]

[21]

[22]

References [1] R. Springenschidt (Ed.), Thermal Cracking in Concrete at Early Age, Proceedings no. 25 of the International RILEM Symposium, Munich, E&FN Spon, London, UK, 1994. [2] P. Acker, F.-J. Ulm, Creep and shrinkage of concrete: physical origins, practical measurements, Nuclear Engineering and Design 203 (2 – 3) (2001) 143 – 158. [3] A. Bentur (Ed.), Early Age Cracking in Cementitious Systems, State of the Art Report of the RILEM Technical Committee TC 181-EAS, Haifa, RILEM, France, 2002. [4] A.G.A. Saul, Principles underlying the steam curing of concrete at atmospheric pressure, Magazine of Concrete Research 2 (6) (1951) 127 – 140. [5] J. Byfors, Plain concrete at early age, PhD. thesis report FO 3:80, Swedish Cement and Concrete Research Institute, Stockholm, 1980. [6] M. Regourd, E. Gauthier, Behavior of cement under accelerated hardening, Annales de l’Institut Technique du Batiment et des Travaux Publics 387 (1980) 65 – 96. [7] M. Emborg, Thermal stresses in concrete structures at early ages. PhD. dissertation, Lulea University of Technology, Lulea, 1989. [8] P. Laplante, Mechanical properties of hardening concrete: a comparative analysis of ordinary and high performance concretes, Research

[23]

[24]

[25]

[26]

[27]

[28] [29]

report LPC OA13, Laboratoire Central des Ponts et Chausse´s, Paris, 1993, in French. M. Laube, Constitutive model for the analysis of temperaturestresses in massive structures, PhD. dissertation, TU Braunschweig, Braunschweig, 1990, in German. K. Van Breugel, Simulation of hydration and formation of structure in hardening cement-based materials, PhD. dissertation, TU Delft, Delft, 1991. F.-J. Ulm, O. Coussy, Modeling of thermo-chemo-mechanical couplings of concrete at early ages, Journal of Engineering Mechanics, ASCE 121 (7) (1995) 785 – 794. G. De Schutter, L. Tearwe, Degree of hydration-based description of mechanical properties of early age concrete, Materials and Structures 29 (7) (1996) 335 – 344. Z.P. Bazˇant, S. Prasannan, Solidification theory for concrete creep: I. Formulation, Journal of Engineering Mechanics, ASCE 115 (8) (1989) 1691 – 1703. F.-J. Ulm, O. Coussy, Strength growth as chemo-plastic hardening in early age concrete, Journal of Engineering Mechanics, ASCE 122 (12) (1996) 1123 – 1132. F.-J. Ulm, O. Coussy, Couplings in early-age concrete: from material modeling to structural design, International Journal of Solids and Structures 35 (31 – 32) (1998) 4295 – 4311. F.-J. Ulm, O. Coussy, What is a massive concrete structure at early ages? Some dimensional arguments, Journal of Engineering Mechanics, ASCE 127 (5) (2001) 512 – 522. J. Sercombe, C. Hellmich, F.J. Ulm, H. Mang, Modeling of early age creep of shotcrete: I. model and model parameters, Journal of Engineering Mechanics, ASCE 126 (3) (2000) 284 – 291. C. Hellmich, J. Sercombe, F.-J. Ulm, H. Mang, Modeling of early age creep of shotcrete: I. application to tunneling, Journal of Engineering Mechanics, ASCE 126 (3) (2000) 292 – 299. C. Hellmich, H. Mang, F.-J. Ulm, Hybrid method for quantification of stress states in shotcrete tunnel shells: combination of 3D in situ displacement measurements and thermoplastic material law, Computers and Structures 79 (2000) 2103 – 2115. M. Cervera, J. Oliver, T. Prato, Thermo-chemo-mechanical model for concrete: I. Hydration and aging, Journal of Engineering Mechanics, ASCE 125 (9) (1999) 1018 – 1027. M. Cervera, J. Oliver, T. Prato, Thermo-chemo-mechanical model for concrete: II. Damage and creep, Journal of Engineering Mechanics, ASCE 125 (9) (1999) 1028 – 1039. P. Acker, Micromechanical analysis of creep and shrinkage mechanisms, in: F.-J. Ulm, Z.P. Bazˇant, F.H. Wittmann (Eds.), Creep, Shrinkage and Durability Mechanics of Concrete and Other QuasiBrittle Materials, Proc. of the Sixth International Conference CONCREEP6, Elsevier, Oxford, UK, 2001, pp. 15 – 25. G. Constantinides, F.-J. Ulm, The effect of two types of C – S – H on the elasticity of cement-based materials: results from nanoindentation and micromechanical modeling, Cement and Concrete Research (submitted for publication). T.J. Hirsch, Modulus of elasticity of concrete affected by elastic moduli of cement paste matrix and aggregate, Journal of the American Concrete Institute 59 (3) (1962) 427 – 452. U.J. Counto, The effect of the elastic modulus of the aggregate on the elastic modulus, creep and creep recovery of concrete, Magazine of Concrete Research 16 (48) (1964) 129 – 138. A. Guidoum, 3D numerical simulation of the behavior of concretes as granular composites, PhD. dissertation No. 1310, Swiss Federal Institute of Technology in Lausanne, Lausanne, 1995, in French. R. Le Roy, Instantaneous and time-dependent deformations of high performance concretes, Research report LPC OA22, Laboratoire Central des Ponts et Chausse´es, Paris, 1996, in French. A. Zaoui, Continuum micromechanics—a survey, Journal of Engineering Mechanics, ASCE 128 (8) (2002) 808 – 816. J.J. Thomas, S.A. FitzGerald, D.A. Neumann, R.A. Livingston, State of water in hydrating tricalcium silicate and portland cement pastes as

O. Bernard et al. / Cement and Concrete Research 33 (2003) 1293–1309

[30]

[31]

[32]

[33] [34] [35] [36]

[37]

[38]

[39] [40]

[41]

[42] [43]

measured by Quasi-Elastic Neutron Scattering, Journal of the American Ceramic Society 84 (8) (2001) 1811 – 1816. P.D. Tennis, H.M. Jennings, A model for two types of calcium silicate hydrate in the microstructure of portland cement paste, Cement and Concrete Research 30 (6) (2000) 855 – 863. R. Berliner, M. Popovici, K.W. Herwig, M. Berliner, H.M. Jennings, J.J. Thomas, Quasielastic neutrons scattering study of the effect of water-to-cement ratio on the hydration kinetics of tricalcium silicate, Cement and Concrete Research 26 (2) (1998) 231 – 243. J.H. Taplin, A method for following the hydration reaction in portland cement paste, Australian Journal of Applied Science 10 (1959) 329 – 345. I.G. Richardson, The nature of C – S – H in hardened cement, Cement and Concrete Research 29 (1999) 1131 – 1147. G.W. Groves, TEM studies of cement hydration, Materials Research Society Symposium Proceedings 85 (1987) 3 – 12. H.F.W. Taylor, Cement Chemistry, Academic Press, New York, 1990. K.L. Scrivener, H.H. Patell, P.L. Pratt, L.J. Parrott, Analysis of phases in cement paste using backscattered electron images, methanol adsorption and thermogravicmetric analysis, Materials Research Society Symposium Proceedings 85 (1985) 67 – 76. S. Diamond, D. Bonen, Microstructure of hardened cement paste—a new interpretation, Journal of the American Ceramic Society 76 (12) (1993) 2993 – 2999. H.M. Jennings, A model for the microstructure of calcium silicate hydrate in cement paste, Cement and Concrete Research 30 (1) (2000) 101 – 116. T.C. Hansen, Physical structure of hardened cement paste. A classical approach, Materials and Structures 19 (114) (1986) 423 – 436. A. Boumiz, C. Vernet, F.C. Tenoudji, Mechanical properties of cement pastes and mortars at early ages. Evolution with time and degree of hydration, Advanced Cement-Based Materials 3 (1992) 94 – 106. P. Acker, Mechanical behavior of concrete: a physico-chemical approach, Research report LPC 152, Laboratoire Central des Ponts et Chausse´es, Paris, 1988, in French. E.J. Garboczi, Computational materials science of cement-based materials, Materials and Structures 26 (2) (1993) 191 – 195. G.Q. Li, Y. Zhao, S.S. Pang, Y.Q. Li, Effective Young’s modulus estimation of concrete, Cement and Concrete Research 29 (9) (1999) 1455 – 1462.

1309

[44] J.D. Eshelby, The determination of the elastic field in an ellipsoidal inclusion, Proceedings of the Royal Society of London A 241 (1957) 376 – 392. [45] T. Mori, K. Tanaka, Average stress in matrix and average elastic energy of materials with misfitting inclusions, Acta Metallurgica 21 (5) (1973) 1605 – 1609. [46] A.V. Hershey, The elasticity of an isotropic aggregate of anisotropic cubic crystals, Journal of Applied Mechanics 21 (1954) 236. [47] E. Kro¨ner, Bounds for effective elastic moduli of disordered materials, Journal of Mechanics and Physics of Solids 24 (1977) 137 – 155. [48] J.J. Beaudoin, Comparison of mechanical properties of compacted calcium hydroxide and Portland cement paste systems, Cement and Concrete Research 13 (1983) 319 – 324. [49] F.H. Wittmann, Estimation of the modulus of elasticity of calcium hydroxide, Cement and Concrete Research 16 (6) (1986) 971 – 972. [50] P.J.M. Monteiro, C.T. Chang, The elastic moduli of calcium hydroxide, Cement and Concrete Research 25 (8) (1995) 1605 – 1609. [51] K. Velez, S. Maximilien, D. Damidot, G. Fantozzi, F. Sorrentino, Determination by nanoindentation of elastic modulus and hardness of pure constituents of Portland cement clinker, Cement and Concrete Research 31 (4) (2001) 555 – 561. [52] L. Granger, Time-dependent behavior of concrete in nuclear tanks: analysis and modeling, Research report LPC OA21, Laboratoire Central des Ponts et Chausse´es, Paris, 1996, 1995, in French. [53] P.W. Atkins, Physical Chemistry, 5th ed., Oxford Univ. Press, Oxford, 1994. [54] M. Avrami, Journal of Chemical Physics 7 (1939) 1103 – 1108. [55] J.J. Thomas, H.M. Jennings, Effect of D20 and mixing on the early hydration kinetics of tricalcium silicate, Chemistry of Materials 11 (1999) 1907 – 1914. [56] K. Fuji, W. Kondo, Journal of American Ceramics Society 57 (1974) 492 – 502. [57] T.C. Powers, T.L. Brownyard, Studies of the physical properties of hardened Portland cement paste, Journal of the American Concrete Institute 18 (1946) 101 – 132. [58] C. Le Bellego, Chemo-mechanical couplings in concrete structures submitted to leaching: experimental study and numerical analysis, PhD. thesis report, LMT-Cachan, Cachan, 2001, in French.

Copyright © 2021 COEK.INFO. All rights reserved.